FSC 7530 WRITING, WHITE AND COLORED JCP D10
Writing Paper (TABLET OPTION) February 1, 1999
Use information: This paragraph is informational only and is not exclusively definitive of the end use.
For face and back offset printing. The 45 g/m2 paper is generally for use on open forms, including multiple copies, one side only.
The 60 g/m2 paper and heavier are used in printing books, pamphlets, catalogs, open forms, etc. Printed matter may include text, line
illustrations, and ruled forms. Halftones and reverse prints may be included on the 75 g/m2 paper for offset printing by simultaneous
face and back, blanket to blanket production. Slitting, pasting, and/or cross perforating are included in press capabilities. When stock
is used on open forms, including multiple copies, one side only, for scratch paper, note pads, tablets, opacity of stock is not a specified
Stock: Groundwood pulp, not to exceed 1 pct. Ruling and writing qualities: Lines ruled and characters writ-
Note: Not less than 30 pct postconsumer fiber. Any percent over ten with ball point and felt tip pens shall be clear cut and free
30 percentage points is encouraged, provided that the require- from excessive feathering.
ments of this Standard are met.
General appearance: Paper shall conform to the standard sam-
Grammage (g/m2) .......................... 45 60 68 75 ple(s) adopted by the Government.
Basis weight: 17 by 22 inches,
500 sheets (pounds) ..................... 12 16 18 20 Color: The paper in the order (or publication) shall be uniform
A tolerance of ±5 pct shall be allowed. with a target brightness of 79 pct for the white paper or as spec-
ified. The color variation shall not exceed DE(CIELAB)=1.0.
Folding endurance: Average, each direction, not less than— For colored stock, paper shall match one of the established
M.I.T. (double folds) .................... 7 8 8 8
Schopper (double folds) ............... 12 16 16 16 standards. Standards are blue, buff, green, pink, salmon, or yel-
low. Colors shall not fade or transfer (rub off) and shall appear
Opacity: Average, not less than even and uniform on the surface of the sheet. Stock shall not be
(percent) ....................................... ............ 83 84 85 2-sided. Color coordinates for selected standards are included in
No individual specimen shall av- Part 3.
erage less than (percent) ............ ............ 81 82 83
Note: This property is automatically waived if paper is used Finish and formation: Shall be uniform.
for the production of scratch or note pads (tablets).
Cleanliness: The dirt count for each side of the paper shall not
Thickness: Average (60 and
75 g/m2 only) (mm) ...................... ............ 0.075 ............ 0.095 exceed 650 specks per square meter. No sample sheet (600 to
Equivalent (inch) ......................... ............ 0.0030 ............ 0.0037 650 cm2 in size) shall contain more than one defect with an
equivalent area of 0.25 mm2 or greater.
A tolerance of ±0.011 mm (0.0004 inch) shall be allowed.
Paper shall be uniform and shall not vary more than 0.011 mm Sampling and testing: Shall be conducted in accordance with
(0.0004 inch) from one edge to the other. standards in Part 2, Government Paper Specification Standards.
Unless otherwise specified, the following is automatically waived when printing or duplicating is to be accomplished on commercial contract
Sizing: Paper shall be surface- and internal-sized suitable for sat- long dimension 813 mm (32 inches) or less shall be considered
isfactory printing on both sides of the paper on high-speed heat- square if the variation does not exceed 1 mm (1⁄32 inch); over
set web or sheet-fed offset presses equipped with continuous flow 813 mm (32 inches); 2 mm (1⁄16 inch).
or brush dampening systems. Rolls: Roll width and diameter shall be as ordered. A tolerance
of ±2 mm (1⁄16 inch) shall be allowed for width and ±26 mm (1
Tensile strength: For roll stock only, average, not less than—
inch) for diameter.
Machine direction (kN/m) ........... 1.3 2.5 3.1 3.5
Cross direction (kN/m) ................ 1.1 1.2 1.3 1.4 Roll winding: Roll paper shall be tightly wound at even tension
Equivalent— and shall not contain more than the specified maximum number
Machine direction (kg/in) ............ 3.4 6.4 7.9 9.0 of splices per roll. The number of splices permitted per roll is de-
Cross direction (kg/in) ................. 2.8 3.1 3.4 3.6 termined by the roll diameter as ordered. On rolls 1,016 mm (40
Color: Shall match the Government’s standard sample for color. inches) or less, a maximum of three splices per roll shall be al-
A deviation of DE(CIELAB)±3.0 from the color standard for lowed. On rolls over 1,016 mm (40 inches), a maximum of four
white and 2.0 for colored stocks is allowed. A color difference 1.0 splices per roll shall be allowed. Splices shall be neatly and se-
DE unit between felt and wire sides is permitted. curely overlap-pasted and made with a repulpable adhesive
which will not permit the splice to separate while passing
Curl: Paper shall lie flat with either no tendency to curl or with through a drying oven maintained at 200 °C. The adhesive may
a curl which can be overcome under reasonable working condi- be applied from a tape form backing, provided the backing is re-
tions. moved, leaving only the adhesive component on the splice. The
Surface: Shall be free from lint, fuzz, or any particles which will adhesive shall not cause the splice to adhere to adjacent laps.
pick, left, fluff, or pile on the blanket under normal press condi- The tails of the splices shall be neatly and evenly removed with-
tions. out damage to adjacent laps. Splices shall be flagged at both
ends with projecting colored markers, not pasted to the splice,
Size and trim: Sheets: Paper shall be furnished in the size(s) or- or otherwise clearly marked.
dered and shall be flat, trimmed square on four sides with clean
smooth edges, and evenly jogged. A tolerance of ±2 mm (1⁄16 Grain: Direction of the grain on flat paper shall be as ordered.
inch) shall be allowed except for sheets 216 by 356 mm (81⁄2 by
14 inches) or less; then a tolerance of ±1 mm (1⁄32 inch) shall be Pressroom conditions: The bulk of this paper will be used in
allowed. Successive sheets within any package shall not differ air-conditioned pressrooms maintained at 24 °C ±2 °C and 45 pct
from each other by more than 0.5 mm (1⁄64 inch). Paper with the ±8 pct relative humidity.